advertisement

Revista Mexicana de Física 42, No. 3 (1996) 343-354 The the9ry of multifractal elasticity: basic laws and constitutive equations ALEXANDER S. BALANKIN Instituto Tecnológico y de Estudios Superiores de Monterrey Camp1fs Estado de México, México 52629 Recibido el 18 de agosto de 1995; aceptado el 29 de enero de 1996 , ABSTRACT.Two basic laws of multifractatelasticity áre formu}ated in géner'al form, leading to a closed system of constitutive equations. This approach allows tó' exp}ain 'íhe elasticity of materials governed by multifractal and hookean medíanisms. It is also noted that for materials of pure multifractal origin their elasti¿ behavior can be used to estímate three first generalized dimensions (metric, information, and correlation) of random (multifractal) microstructure. With the introduced new framework, classical formulas for rubber-like,and spring-like elasticity are derived as well as constitutive equations for superelastic materials. The theoretical resultsreasonably agree with.experimental data and computer simulations reported in the literature. . ," RESUMEN.Se formulan"en forma;general dos leyes básicas de la elastfeidad multifractal, que conducena>un sistema de ecuaciones constitutivas. Este método permite explicar el comportamiento elástico de materiales gobernados por mecanismos multifractales y /tookeanos. Se discute que para materiales de origen puramente multifractal, su comportamiento elástico puede ser empleado para estimar las dimensiones métrica, de información y de correlación de microestructuras estocásticas (multifractales). En este nuevo marco de referencia, se derivan las fórmulas clásicas dé elasticidad rubber-like y spring-like, así como las ecuaciones constitutivas para materiales superelásticos. Los resultados teóricos obtenidos coinciden razonabÍemente con los datos experimentales y con las simulaciones computacionales reportadas en la literatura. PACS: 03.40.Dz; 62.20.Dc; 64.30.+t In the last ten years the theory of materials with randol!l (fraetal 01' multifraetal) mierostrueture has beeome an attraetive tapie in mechanies ando physics of solías [1-6]. Statistieal properties of a multifraetal are eharaeterized by a speetrum ofgeneralized dimensions dq [1]. Generally, the generalized dimens!pn dq = O is equal to the metrie (fractal) <iimensionevaluated by means of the box-counting algorithm, i.e., do = dF, which for multifractal structureis greatcr than its topologieal dimension dT, but smaller than;' 01'equal ", to, the topologiealdimension d of the enveloping Euclidean spaee, i.e., dT < dF ~ dj the generalizeddimcnsion of arder q = 1 is equal to the,iiíformátion dimension dI = d¡ j and the dimension dq = 2 is equal to the eorrelation integr~l exponent de = d2, algo called eOÍ'relation dimension. Acrogel, eolloidal aggregates, polymcrs, some types of composite materials, porous media, cte. llave a multifractal structure in a' wide range of spatial scales Lo < L < Lu [1-3]. ALEXANDERS/BAL~NKIN ~ ~ ~ . - k'ei~fou.rdifferent';typesoéelastlcity" [4]1a.r~~pioadlyus~d foromodeling elastic IJ}"'~' f !ll,.teria1s'with plultifr&ftaI, ÍJÜt' ~ure:' 1t~elastiC'1ty'ot" ~J1ergetic nature ntinuiÚn;'crystaIs, "polYcrYStiUs';"' e ased olÍ:tne generaU~;Hooke'8 la.wj 2) entropy eI~ticity(elastomers), b~eponGáus~)an statiSt!cS <tíeleme~ts(mjcrofstru~túre¡ a¡ñYJ>er':and sup~relasÜdty, which are described by usiÍlg plienomenologicaI:modelsfor elastic ~poientialj and 4) spring-li~e elast~city (191lgpoIymer Cháirls, foamB, Borne~tru<:~ bella (elaSt ~,.~ .'," o" o~"", ~ . turaI composjtes, et~.) b' on tpe:em eras' . .,' .' bas'~ o JricáI form~la fol: spril!g~~o;. '.' .::" In:th~ se~Qfour wo. :,;gr~;yp~'of fract.~elasticity;(seeaJso;r~iewg15,6 ogI fráCf "o. , d multifr~a.t . , , . sugieStiji'that::¡siheo:rqulti- '. e)l.ávior forUl~térialSwith". .,aY "d~ ,'~ ~""Qr 41co~ '~h~ gidilJa s oftéVe,r.~l .~'deforníatt9h ultifractaI . /~() ;pos~te<l'P structures. --o :~. '..0 .~ o,. -"'~;::,., .,' -<,o o lJi, 'thi~attic1e' we~"giv ~''g~ri~¡átdormulationJ~r t~t l~!is o(~uiti.fractaI " .!le in ofeoii~titü~iv~'fquatioIÍs;::,illO~.be sñ()\ynth~t elast{~it ' tbe-.entr - ike e ." super.,.and 4Yí>erelasticit~;~("¡::'8pring-!r tici~Yc. aie ~he spj<:ifi~" of the m~ al ~ .. .¡he.generalization oí tlte d opedíi.theory \vhitili-elJm1>i the multif¡'~ lid: fÍu}déWo es .1s'a:ls~ di$cUSSed. "0B_~la\vs of.>reyersibledeformati~el~icin 'tOi'mülat~ inthe >' o fóllt')ws:."< geneJ'aI'fo~mas " ",;c;"~;""': 1) ~When the~~emiil ¡; F¡s'ííppliea ~JormatÍlin8 ocC.urlength,scale '. ~pends oJP,; Th~;,:'Ut o valid, obeys reíatioJi~' o' , o'01 ~n' éxternal c8treS$:¿re-ads tp tn,e ap1Jé".;ante oj ~,,~ unique netOcharoc~tr¿~~1 Ir this-Jawis .~, ttl'iiit't!laitic 'is'~jjio;ctiil;objed, bellond;;~ain:chns~ length,llJh,icJ.', th~LE~~;:2'",.., .;,' ; oo." ~,': . ;; the secon9':l~w ott~9dyifámics-it o ..' , "1 ,F~.~ ( ) 'IJLF . ."~~~ ,°; aw t au, J ;:~;f1ll-/ "'"' " ".,:': as C-i~ ' ( ) ) 'T,'-'1' IJE; "o foJlows i1lat)1í~ force ."C:"¡:, '~ "' ,o"'~;,~,,:; , (l} T' . Tbe fi!8ftermon ,th~ right of Eq. (1) is,eyidently the energy component of internal, forces,~"'and the secondter~s is theentropic coIBP<:ment",o;, ",,'" 2) The reversible !-eJorma~io'MQl multijractaa are homeom~rphi~; , , , : , affine. It jadear that ah°Inoe~orphi9 deform,ation(one-to-oneami ontót formatiori) does not ~gethe mettic'(fractaI) dimenl)ion,ofa deformed multifracta1..Moreover in Ref. (15] it waSshown that thel'e are' gesmthe informátion:land córrelation dimensions a.f. t:eI"'aJfi~etrán~fórmation'( de )~!:~f mult,ifl'act'fsthl~t ure,whi}ec.t~e limiti~~!alues , , ;:e;' " ,~:::-:", " tyPés o'{elastic be.1ui,~' 'e'b¡.sed~ó1i':;différent1>henom~íiologicaj-la\~ perimesl81 tactsf~dJead to dJft'ert( ijutive equations. '"'"' , ",'¡;~':f., "1~"'¡': , , " , , ,2 1'he'~initiaI IOOtphology'Q.fí~muJt, ,'. ta1r~ ~ ., 344 ',be chaiactéOzed;;,by ,~ oJ}e;or;¿m~re:,.gtb: sCalePara.IJ.1eteFS'Lior dOE!Snót have them~. 'the fitst casththe:.ct:.may"ha~rphXsi:caJ signific,an~esuch as characteristi~ d~~nsion of-blob~ in' a polymer, ch!Ú'~teristic oSi2:Et'of cells" °L meandistantebetWeenineIu .' "', QpipQSitematerial, cbaracteristii:rádius6f<;9rrelations in a ,: random network'and aerogél, , foll~ivs from the'lá.w p'Ostul~ted,'abo~, onfY:one of the~set of scaJe parametérs Li (or the\r invariantcótnbiriation) depenas on,ctlie'exíernal forceS. If theinitiaJ mllltifractaJ gttucture has nostále pa.tain~teistken the physical rñéariingóf LF. is the'Characteristic lengthabOve which deformations occur. ': ' THE THEORY OF MULTIFRACTAL 345 ELASTICITY:... 'oí generalized dimension spectrum, e.g., doo and d_oo,after affine.transformation in general differ from those for initial multifractal structure. Therefore, if the second postulate (law) is valid the metric, information, and cmrelation dimensions of deformed multifractal structure are constant. The mass density p of a material with multifractal microstructure generally depends on the length scale,L [3]. Dimensional" analysis implies the following general' functional relation: ,, P=PoiJ! ~c LF ( ) (L'L ) =POiJ!Ac,Af, (2) where W is a dimensionless function of its dimensionless arguments Ac = ~c/L and~Af = LF / L; ~c is the correlation length of multifractal (micro)structure. It is well known that within the bounded interval LF ~'L...~ (3) ~c + the,mass density of multifractal structure p(L) obeys á power law behávior [3}'{According to inequality(3) the secondargument of the dimensionlessfunctioniJ!(Ac, Af) is small (.\f ~ 1); so that ati'the asymptotic self-similar state we can apply to the function iJ!a sqaling (incomple'teself-similarity) representation [16] P0F= PpX¡c~ 'IjJ(Ac), Q= d - dF, (4) where 'dF is the fractal Emetric, box-counting) dimension'pf the multifractal ami 'IjJis a dimensioñalessfunction of ~'c; Notice that,p possessscaling behavior (4) in"the initial'stat~ of the multifractal structure' as well aw"after any deformation of this structure, but~c and dF, generally speaking, may be differentbefore and after the deformation. However, according to the first la~9f reversible deformations, only the characteristic length LF changes after elastic (reversible) deformation of elastically isotropic multifractal, so that ~c must be constant. Furthermore, elastic deformations "are h<:nueomorphic by definition and thus do not change the metric dimension dF of the deformed multifractal, . so that the scaling expqnent Q is algo constant. By this means, the mass density of elastic multifractal structure arte! its reversible (homeomorphic) deformation caused by different external force§ Fl and F2 is equal to p(F¡) = POAfl'IjJ(Ac)~nd p(F2) = POAf2'IjJ(Ac), respectively. Hence the ratio p(F¡)/ p(F2) is Jlot ¡dependent on neither the varia15le ICl~gthscale ? nor..the correlation length ~c and scales as . " p(F¡) p( F2) = Afl -(): = ( ) Af2 LFl ( ) -(): = AFO:' L F2 T=const Q= d - dF, (5) i. e. the relation governing the change in the mass density p of elastically deformed multifractaJs is similar to the relation that governs the change in the ma,ss d~nsity because 346 ALEXANDER S. BALANKIN of the geometric change in the dimensionalities of (multi)fractal structure3 (within the interval (3)!). It immediately follows form Eq. (5) that under uniaxial tension (compression) the change in the dimensionality .of multifractal structure in the direction of external force Fx, which is Ax = Lx/Ix, is accompanied by the change in the lateral dimensionalities of deformed multifractal structure in orthogonal directions of the surrounding d-space with A¡ = L¡/l¡,wherei = 1,2, ... , d - 1. The lateral deformations A¡ are related to Ax = AF as Ai = Al. = A;Vf' = AFvF, i = 2,3, . . . , d, (6) where lIF is the transverse deformation exponent.4 Substituting (6) into Eq. (5) we obtain a = 1 - (d - l)vF, so that lIF ~ In Al. - dF --1 . In AF - d - 1 (7) Therefore, if the first postulate (law) is valid, the transverse deformation exponent lIF of an elastically isotropic multifractal is defined uniquely by its metric dimension.5 The data of Table 1 demonstrate that the results of calculations by the analytical formula (7) agree well with results of computer simulations of the elastic properties of twodimensional percolation networks near a percolation threshold (see algo the Appendix), as well as with the experimental data for aerogel SiO2 (which were obtained in the studies of the longitudinal and transverse elastic waves propagation), rubber, and a strongly twisted nondeformable polymer filaments. At the same time, it must be emphasized that Eqs. (5) and (7) are not valid for materials obeying conventional Poisson's effect, or, what is equivalent, the generalized Hooke's law. For such materials the correlation length (c is equal to the sample size in the direction of applied external force, i.e., (c ==Lx; so that (c and AC = Ac1 Ac2 = (8) ~Cl (C2 must change .after deformation. At the same time, for an elastic continuum Ar = O and AF ==1, while for a regular elastic lattice Ar = a/ ao (a and ao are the interatomic distances before and after elastic deformation, respectively) and AF = Ac.Hence, for materials obeying Poisson's effect our first postulate is not valido 3 Notice tbat formerly this fact was postulated as the second'law (see, for example reviews [5,6]). In fact, as is shown above, Eq. (5) is a direct consequence oí the first law and oí the homeomorphism oí reversible deíormations. 4 Notice tbat the exponent of lateral deformation~ lIF -In A1./AF is equal to the Poisson's = ratio v = -.JiA22 - li7iAll - li only in the limit of infinitely small strains é:¡¡= ~ « 1. At first glance, it is surprising that lateral deformations are independent of the detailed geometry of deíormed multiíractal. Notice, however, that similar situations (power law distributions of stresses and strains with exponents which are a function only oí Poisson's ratio) are common within singular problems in the classical theory oí the elastic continuum obeying tbe intermediate asymptotic behavior (see, for example [17,18]). 5 THE THEORY OF MULTIFRACTAL 347 ELASTICITY:... TABLE 1. Comparison oí Poisson's ratio v, calculated using analytical relationship (7), with the computed values, based on two-dimensional elastic random networks, and with experimental data íor aerogel SiOz, strongly twisted nondeíormable polymerfilament, and rubber. Properties Two-dimensional random network oí size L x L near the percolation threshold (~c - correlation length) L/~c Connectedness oí random network Fra.ctal dimension oí elastic backbone dF ~ I/F, Eq. (7) Poisson's ratio (results oí numerical simulation and experimental data) -~ 00 L/f.c ...,..o Elasticity oí network is determined by danglingbonds Bonds, determining elasticity oí network are multiduplicated Dimension oí geodesic line, dmin = 1.1.:i:0.02 dF = drb, drb = 3/4 [29] [29] 0.1 :i: 0.01 -1/3 0.08 :i:0.04 [28] -0.33 Strongly -twisted nondeíormable filament Rubber Fractal cluster Monomer Polymer network dF, measured by smaH;angle neutrÓn scattering and molecular adsorption [31]: 2.3:i: 0.1 Dimension oí red bonds, . dF= dmin, Aerogel SiO2 :i: 0.01 [28] Dimensiori oí selí-avoiding random walk: d.-a = 2 [29] = dF 3.00 :i: 0.04 [25,26] 0.15:i: 0.05 O 0.50 :i: 0.02 0.12:i: 0.08 [30] O [27] 0.50 :i: 0.01 [22] ~-<~ Furthermore, the."metric dimension of an elastic continuum as well as a r,egular elaStic lattice (dp ==dq for all q), which can be considered as a limiting c¡;tsesfor multifr~~tal structures, is equal to the topological dimension of structure dT; so that - '" d, dp =d{ - 1, a= O, dT = d { 1, dT = d - (9) 1. Now, it is easyto understand that in the case of an euclidean elastic structure obeying generalized Hooke's law the dimensionless function 1/Ip(Ac) = 1/I(Ac1)/1/I(Ac2)scales limit of infinitely small strains!) as 1/Ip = ( ) ~Cl ~C2 (in the -f3 == Lx(F¡) -f3= Xc/, ( Lx(F2) ) (10) where {J = 1 - (dT - l)v. The relation for the conventional Poisson's effect Ejj ,= l/En (see footnote 4) may be derived by substitution of Eqs. (10) and (6) with dT = d in the general relation (4). Therefore, in the general case of an elastic multifractal structure, the lateral deformations of which are governed bythe combination of lateral deformations of the Ínultifractal nature with those associated with the conventional Poisson's effect, the scalingrelation (5) 348 ALEXANDER S. BALANKIN can be generalized into p(F¡) - A-(d-dF)~{dT-I)v-1 p(F2)"- F k,G . (11) It should be emphasized, that relation (11) is valid only in the limit of infinitesimally small strains Cii = J!A~ - 11~'1! Now, if a mtiltifractal structure possesses Poisson's effect with Ae = AF,the transverse deformation exponent is equal to d-dF lIF=lI- ([ (12) 1' This relation governs the lateral défórpiation of the multifractal"is"wéll as the Poisson's nature. Below we will corisid~r only the elastic multifractals'.reversible behavior, whicli"'is governed by the two laws postuláted above. The lateral deformations of such'a structure nave apure metric origin (Ae ='1)6'and are governed by the metric dimensionof the structure (see Eq. (7)). Looking back at the two proposed.laws oheversible deformations for multifractal structures, we see that we need to know the changes in the éntropy and;~internal energy as functions of deformations before the closed system of constitutive equátions can be obtained. Using the definitions of the infórmation'and correlation dÍlpensions and theif scaling properties [1,2] with'rehttions (1), (5) valid, it is easy to show that the changes in the thermodynamic entropy ~S(Ai) and in the internal energy'U(Ad during the reversible deformation 'oí an elastic mtiltifractal in d-:-dimensional splce can be represented in the "', ~~ w T ~S = -C2 ( t ~=l A1r - d) , (l3) and ~U = -Ct(A~C - 1), ae = d - de, (14) respectively. Here CI and C2 are constants (noti<;ethat parameters CI and C2 can algo be determined for any detailed modél of the~structure [19]). Substituting (13) and(14) into (1), and using relations (5)-(7) we can derive the relationships between external force Fi and relative deformations Ai of multifractal structure. For example, in the case of uniaxial deformation (tension 01'compression) wf obtain FI = C2{dIAfr-1- dddF - (d - l)]Aidr[dF/(d-I)-I]-1 -"cIC2 (d - dc)Af-dC-I , . } . (15) 6 It is pertinent to note that in th~ case AC = AF and 11= l/(d-l) Eqs. (11), (12) are equivalent to Eqs. (5); (7), so that all results considered below are algo valid in this more general 'case. THE THEORY OP MULTIPRACTAL ELASTICITY:.., 349 According to the dbvious condition F(>'i = 1) = O,it followsfreIDEq. (15) that Cl C2 =d dId dp <d - de - (16) P, so that 7 Fl = C2dl{>.f¡-l - [dp- (d - l)]>'ld¡(dF/(d-l)-l]-,~- (d - dp».f-dc-l}~ (17) Thus behavior patterns of elastic m:ultifra<;tals (for which"two laws pdstulated above are valid!) are completely determined by the metric, information, and correlation dimensions. Moreover, it is easy to see that in the limit of infinit'ely small strains, Eqs. (17) and (7) can be,generalize~ by using Eqs. (11) and (12).' In the case of monofractal structure all generalized dimensions areequal to the. metric (fractal) dimension, i.e., dq ==dF = dI = de [1], and Eq. (16) results in the equality Cl c-..2 (18) = dFf..."' So that, Eq. (15) may be rewritten in the forro Fl = Cl {'>.fF-l - [dF- (d - l)]>'lvFdF;l - (d - dF»'1-l}. (19) The stress 0"11is related to the force Fl (.xI) by obvious equation 9':11= Fl>.t-a, wliich by using Eqs. (7), (19) may be written in theform 0"11 = E 1+6vF+4v~ " 1+4vF [ (.xl -1)-2vp(>'1 -1- 2 2VF,-1)], (20) where E = ({)O"11/8E:11)r is the Young modulus. It is easy to see that, within the limit ofinfinitesima}ly small strains, jé:lll = ".jl>.it- 11 « 1, Eq, (20) leads to its classic counterpart for elastic continuuin. Thus~ fOl'monofractal structure we llave Cl = 2(1 + vv)C2 = (1'+ 6VF f 4¡)~')E. ,Similarly, we can derive the relations O"ij(>'k)for n-axial deformation of an elastically isotropic monofractal in the d space. The pure shear is essentially a biaxial loading under the stresses 1711ande0"22such that there is no change in length aloi\g{~econd direction, i.e., >'2= 1 (see Ref. [2'0]). Therelationships between the elastic moduli, i.e., Young'sm08ulus E,'she~r modulus G, and balk modulus D, and Lamé cocffieicnts >.,J.lof elastically isotropic(mono!)fractal, - 7 In Reís. [5,6] we llave conjectured that íor an elastic multiíractal d¡(d dp) = de(d - de). This conjecture was made in the spirit oí the Dirac's maniíest tlyit ~a physicallaw must possess mathematical beauty". However, there is no experimental evidente in support oí thisconjecture. In this sense the Eqs. (16) and (17) are more correct ~han the related equations in Reís. [5,6]. 350 ALEXANDER S. BALANKIN which are derived by analogy to the derivation of the corresponding relationships in classical theory of elastic continuum [20], are the following: E B = d(d - dF)' G = E(d - 1) 2dF ' 2 B = >.+ "d/t. (21) Notice that these relations differ from those which were conjectured for elastic fractals by Bergman and Kantor [21]. On the other hand, substituting Eq. (7) in the Eqs. (21) we obtain expressions that' for d 7" 2 [nd d = 3 are identical to those for two- and threedimensional elastically isotropic continuum! ClassicaLformulas for rub1{er-likeelasticity [~2] E = E3 (>'l' - >'12), (22) >'2 = >'3 ==X¡;1/2(p= const), may be -derived within a framework of Eqs. (17) and (5)-(7) for multifractals obeying = d = 3, dF and dI = 2. Notice that the condition dI = 2 is assoti~ed with the Gaussian statistics [7,23], which is used in the classical models of rubber=Íike el{tsticity [22], while' the equality dF = d = 3 is the condition of incompressibility (see Eq. (5~), which is algo assumed in the classical theory [22]. In fact, however, calculations based onEq. (22), with the vatue of E adjusted by fitting, are in reasonable agreement with the experiments only in the range of relatively small strains (>'i < 1.2) [22]. Traditionally, the refinement of the relation (22) is;made by phenomenological modifications of the entropic theory, 9r by using empirical mod,els for the elastic potential [22,24]. At the same time, elastomers are known to llave fractal or multifractal microstructure [3,25,26]. Therefore, it is natural to describe rubber elasticity of polymers by using the results of the concept of multifractal elasticity discuss~d above. Generally the generalized dimensions of polymer networks swelled in a good solvent are within the range 2 < dq ~ 3 [3,25,26]. Assuming in the first approximation that dF = dI = de and substituting Eq. (7) intp E,q. (19), we,obtain the relationship between the nominal stress Fl and the strain factor >'1In the case of uniaxial tension (compression) of an elastomer in the following fo~m: = F 1 E 1 +6/JF +A/J~ { >.1+2//F - 2 ~-1-2//F(1+":F)- ( 1- 2 1 /JF 1 /JF » .-2//F .. 1 }, (23) which was first derived in our work [7¡by other l11t1ans.8Notice, that behavior (23) differs from (22) even in the limit of incO,mpressibly defOl:méd materi~l,whcn Eq. (23) r~dúces to the formula . F2 .. -i. E >.2 - >.-2.5 =_ ), 4.5 ( 1 1 .- (24) 8 We emphasize that Eq. (23)' is a lil11itingcase oí the general equation (19),which gives a richer set oí various behavior patterns. ~ THE THEORY OF~ULTIFRACTAL ELASTICITY:... 351 obeying the experimentally established ~ymptotic (see Ref. [22]) El <XA~, when Al» 1. It was shown in Refs. [5-11] that thei~"talculations based on Eq. (23) agree well with experimental data.,for rubbers without any~adjustment of parameters« except E) right. up to Al = 7. The nonlinear stress-elongation asymptotic for superelastic networks [27], O"U <X A 1/3 1 , P5) is a special case of constitutive e,guations (17) and (7), which is valid for multifractal structures possessing . for example dF = dF + dI - d = 1, (26) 2, d ~ 3, dI = 4/3. The basic relation of spring-like elas~icity [22V E = E(A - 1) (27) mar be algo derived from. (17) and (5)-(Z) in the case of multifractal structures for which . dF = dI = 2 (d = 3). Furthermore, the pseudo-elastic, super-elastic, and l'!lbber-li~e behaviór of alloys ,with thermoelastic martensitic transformation [3] can bealso evaluated within a framework of the multifractal theory'of elasticity.9 Hence the proper regard for the real morphology allows an adequate description for the behavior of a reversible deformed material with fra<;talormultilractal microstructure. Considereg, examples revealed that two laws of reversible deformations' of multifractal structure, which are postulated in preseIlt work, are valid at least for some classes of materials with (multi)f~a~tal (micro)structure. Wechope this work will stimulateexperimental research along this Hile. We expect that these investigations will support our concept of multifractal elasticity. If so, experimental data on elastic behaviorcan be used to estimate the metric, information, and correlation dimensions of the (multi)fractal microstructure. ACKNOWLEDGMENTS Theauthor is grateful to G. Cherepanov for usefuI discu§siol1s.The courtesy and suppor,t of the st{l.ffal1d faculty of Materials Research Cel1ter at Mol1terrey Ul1iversity of Techl1010gy, and especially, A. Bravo, are gratefully ackl1owledged. 9'This tapie will be considered in moredetails in a forthcoming papel'. >;. 352 ALEXANDER S. BALANKIN ApPENDIX The percolating network i8 a fundamental ,model ,for describing geometric,!:l fe.l:tturesof random systems [2,29]. There are two main,.kinds of percolating networks: "Bite" ano "bond". To create a site-percolating network,~~ach inteJ;,section (site) of an initially pre'pared d-dimensionallattice is occupied at random with probability p. Sites are conneCted if they are adjacent along a principal direction. In a bond-percolation network, all sites are initially!occupied ano, 150.ndsaJ:~"occupied randomlYt;with probability p. At a critical (different) concentration p = pc (pc algo depends on the dimension ano symmetry of originallatÍice), both site ano boqd percolation exhibit a single, infinite cluster spanning all space. - When the occúP<1tionprobability pJs less than pc, there are only finite clusters, whereas if p > pc anDinfinite.cluster is pieseht as well as finite clusters. The cluster 'both at pc ano away from pc are characterized by the nuniber of sites, s, in tHe cluster ano by the radius of gyration, Rg(s), of the cluster. Over what distances are occupied sites connected? The connect~dness length (c is defined ~s the average root mean square distance between occupied sites that belong to the same ano finitf. cluster. This connecte~nes~le'9gth is ,algo called the correlation length. The lower cutoff;lscale characterizi!lg the,percolátion cluster is the length a that forros the lattice spacip.g'oftlÍe origiriallaHice. For the problem of the"electricáJ condut'tivity of ahndom resistor Iletwórk ano transport dynamic properties, anotller object isrelevant: th~ cc"backbone"of an ihfinite percolation cluster [29].'Fhe backbone is definedas the network ofunblocked connected bonos, through which one can go to infinity by at'least two nonintersectingpaths. In 'bther worn::l~,tgé backbone is a set of bonos, through which~ele"ctric current would flow were a.votta~e applied to the cluster at infinitely remote efectro'<:les.:::rherest:;6r the Clu.st~ri~refhre<l to as a collection of "dead" 01'','d~ngling ends". A dangling end cah be"disconne~ted"frómthe cluster by cutting a single bond. In random resistor network near~the p~rcolation threshold, some bonos carry'the highest current. These bonos forro the set of single cohnected bonos of the backhone. This set qfbond}3were called "red bonds" (when one red bond is c~ut, the current flow stops). 'The rest of bonos of the backbone is the "blue bonds" (Blue bonds carry current, btit when'a blue bond is cut, the resistance of the system only slowly increases). Anbther important concept is the minimalor "chemical",path between""two points of a backbone, which is the shortest path between th~ two points. The shortest path between the sites i and' j realizes along the "geodesic lipe"" ano 'cahbé d~fi'ned as the minimal number of steps'by wliichwe can reach j from i, witlf'l'estriction to existing paths between connected sites. This is termed the chemlcal distance Lche~ (notice'that it is not the same as the linear length measurcd between the two points ano referred tú as the "Euclidean. distance" ). For any length scale L » (c, a percolating system is macroscopically horn<fgeneous. But for a ~ L ~ (c, the system possesses statistical scaleinvariance ano may be' referred to:as afractal or"multifractal object, all properties ofw.hich obey a power law dependehce on its characteristic linear size L [29]. For exampl~/the total mitn:ber of bonos (01' sites) . of the cluster scales as NcI '" Ldcl, ~ where del'Is' the fractal dimension of the cluster; the total number of backbonc bonos scales as N'bb '" V{bb; thg number of red bonos Nred scales with L as Nred '" LDrb. The chemica1 dimension dchem is d~fincd from the relation THE THEORY OF MULTIFRACTAL ELASTICITY:... 353 Nchem '" L~h~;;' The chemical length scales with Las Lchem '" L1min, where the fractal dimension oí géodesic line dmin is equalto the'l'{Ltio del dchem' / Recently, there has been a considerablé interestin thé elastié" properties of percolat... ing random networks [21,28]. It was found that for elastic prbblem the critical value of occupation probability PCel diffe.rs from pc [32]. For example, for percolation on the twodimensional triangular lattice pc = 0.3473, whereas PCel= 0.58 [32]. Hence .the elastic backbone which govemscelastic behavior of percolating network CaIgodiffers from backbone,govemed electrical resistance. Among the surprises tliat *were uncoyered was the phenomenon of a negative Poisson's ratio'ÍI of percolation network of size L « ~c near the percolation threshold (L ~ a) [28]. It was algo found that the Poisson's ratio is sensitive to the precise value of L/~c, changing from -0.33 when L/~c -+ O to about +0.08 when L/~c -+ 00 (a zero Poisson's ratio was found for L/~c ::=0.2) [28] The most im- portant result of the refered works is that the limiting values of v (namely v(O) = -0.33 and v(oo) = 0.08) are independent of the elementary (microscopic) force constants of the bonds. This give the rige to describe the elastic behavior of sutIl networks within a framework of the theory of multifractal elasticity (see Table 1). REFERENCES 1. T. Vicsek, Fractal Growth Phenomena, London, World Scientific(1992). 2. A.S. Balankin, Synergetics 01 Delormed Solids, Moséow, Department of Defense USSR press (1991). . 3. V.S. lvanova, A.S. Balankin, l.J. Bunin, andA.A. Oksogoev, Synergetics and Fractals in Material Scíence, Nauka,.Moscow (1994). 4. G.P. Cherepanov, A.S. Balankin and V.S. lvanova,. in A Topical Encycl()pedia 01 Current Knowledge Dedicated Alan Arnold Griffith, Edited by G.P. Cherepanoy, Krieger, Melborne, U.S.A. (1996), 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. . A.S. Balankin and P. Tamayo, Rev. Mex. Fís. 40 (1994)506. G.P. Cherepanov, A.S. Balankin and V.S. IvanOva, Eng. Fracture Mech. 51 (1995) 997. A.S. Balankin, Sov. Phys. Tech~ Lett. 17 (1991) 632. A.S. Balankin, Dokl. Russian Academy 01 Scí. 319 (1991) 1098. A.S. Balankin, Sov. Phys. Dokl. 37 (1992) 379. A.S. Balankin and A.L. Bugrimov, Polymer Sci. 34 (lQ92) 889. A.S. Balankin and A.L. Bugrimov, in Abstr. XXVIII Int. Congr. Theor. and Ajipl. Mech. Haila, Israel, August 22~28, 1992, lut. Union Theor. and Appl. Mech. Press, Haifa (1992) 17. A.S. Balankin, Phys. Lett. A210 (1996) 51. A.S. Balankin, Sov. Phys. Salid State 34 (1992) 658. A.S. Balankin, Phys. Rev. B 53 (1996) 5438. A.S. Balankin, J. Phys. A (in press). G.l. Barenblatt, Similarity, sell-similarity and intermediate asymptotics, New York, Consultant Buerau J1979). G.P. Cherepanov, Mechanics 01 Composite Materials, Moscow, Nauka (1983). A.S. Balankin, Sov. Tec~. Phys. Le~t. 175(1,,991)229; 391. S.V. Panyukov, Sov. Phys. JETP71 (1990)$372. . A.E.H. Love, A Treatise on the Mathematical Theory,pl ElO,stícíty, Dover, New York 01.944). D.J. Bergman and Y. Kantor, Phys. Rev. Lett. 53 (lfJ84) 511. L. Treloar, The Physics 01 R1,bber Elas.,ticíty, Clarendom Press, Oxford (1975). C.E. Puente, Phys. Lett. A 161 (1992) 441. ..~'" 354 ALEXANDER S.BALANKIN 24.~S. Edwards and T. Bilgis, Rev. Progr. Phys. 51 (1988) 243. 25. A:M. Aharoni, in Synthesis, Characterization, and Theory 01 Polymer Networks and Gels, edited by ~~M. Aharoni, Plenum Press, New. York (1992). 26. M. Kallala, C. Sanchesand B. Cabane, Phys. Rev. E 48 (1993) 3692. 27. 28. 29. 30. . S.P. Obukhov, M. Rubinstein and R.H. Colby, Macromolecules 27 (1994) 3191. E. Duering and D.J. Bergman, Phys. Rev. B 37 (1988) 9460. M.B. Isichenko, Rev. Modern. Phys. 64 (1992) 961. M. Gronauer, A. Kadur and J. Fricke, in Proc. 1st Symp. Aerogels, Wurzburg, Germany, 1985, Springer- Verlag, Berlin (1986). 31. B.M. Smirnov, Physics 01 Fractal Clusters, Nauka, Moscow (1991). 32. S. Feng and P.N. SeD, Phys. Rev. Lett. 52 (1984) 216.